IOSR Journal of Applied Chemistry (IOSR-JAC) e-ISSN: 2278-5736. Volume 4, Issue 4 (May. – Jun. 2013), PP 01-04 www.iosrjournals.org
Optical Properties of (AR) Multilayer Thin Film for Solar Cell Application C. Gopinathan, M. Kavitha and P.Pandi P.G. and Research Department of Physics, The Madura College, Madurai-625011, India
Abstract: We have been prepared Semiconducting oxide material like TiO2, SiO2, TiO2-SiO2 and TiO2/SiO2 thin films for taken different composition by using hydrothermal method. All these elements were deposited on the glass substrate. In this films are acted on the p and n type working with the majority carrier are recombination of electron and hole .This material is N type but it will acted p-type Ti and Si. Thin films were Characterized by scanning electron microscope (SEM), X-ray diffraction (XRD), and UV. From the UV Studies we have analysis the energy gap (Eg), refractive index (n) and extinction co efficient. Keywords: TiO2, SiO2, TiO2-SiO2 and TiO2/SiO2 thin films, XRD, UV and SEM
Metal oxides, such as TiO2, SiO2 are materials with high surface areas that exhibit exceptional chemical reactivity compared with commercial metal oxides. Metal oxide nanoparticles may potentially be inexpensive alternatives to carbon nanotubes with superior properties for many applications including catalysis, separation, gas storage, energy conversion, drug release, sensing and environmental protection, and biocompatible nanocomposites. The modified form of TiO2 composites such as TiO2-SiO2, TiO2/SiO2 are interest for their potential application, such as electrolytes in dye-sensitized solar cells, anti reflection coating, photocatalysts and so on [1-7]. II. Materials and Methods For preparation of TiO2-SiO2 as precursor solution, Titanium (IV) isopropoxide (TTIP, SigmaAldrich), Sodium Meta silicate, Ethanol and Hydrochloric acid were used as raw materials. The TiO2 was produced by mixing of TTIP and ethanol in the ratio of 1:5. This solution was stirred under 0˚C (ice bath) for 6hrs.The resultant solution was transferred into the autoclave, and aging, annealing temperature are given below the table1.1. The SiO2 was produced by mixing 0.1M of SMS (Sodium Meta Silicate) and 20ml of ethanol.
Table.1. The aging, annealing temperature Samples TiO2 SiO2 TiO2-SiO2 TiO2/SiO2
Stirring temperature(˚C)/hrs 70/6 70/6 70/6 70/6
Aging temperature(˚C)/hrs 120/48 120/48 120/24 120/24
Annealing temperature(˚C)/hr 300/1 300/1 300/1 300/1
III. Result and Discussion 3.1 Structural analysis: In hydrothermally prepared TiO2 (Fig.1a) the peak positions and their relative intensities are consistent with the standard diffraction patterns of srilankite-TiO2 (JCPDS card # 23-1446). It has a main peak at 31.3° corresponding to the (111) plane. The peak position at 26.5° and 31.3° are in accordance with the TiO 2 srilankite phase. The lattice parameter of the pure TiO2 [(orthorhombic) a = 4.55 Å; b = 5.46 Å c = 4.92 Å] are also in accordance with the reported value (JCPDS card # 23-1446). Similarly TiO2-SiO2 (Fig 1b) and TiO2/SiO2 (Fig.1c) thin film was prepared by the hydrothermal method. The peak position confirms the deposited elements. TiO2-SiO2 the peak positions and their relative intensities are consistent with the standard diffraction patterns of brookite- modified TiO2 (JCPDS card #03-0380) and also brookite- TiO2/SiO2 (JCPDS card # 291360). From the Fig.1b. the peak position (8 6 0) corresponds to the SiO2, (1 1 1) and (1 2 1) corresponds to brookite- TiO2. Form the Fig.1c. the peak value ( 1 1 1 ) corresponds to the glass substrate, and ( 2 2 0 ), ( 0 2 2 ), ( 0 3 2 ) and ( 1 2 3 ) corresponds to the brookite - TiO2 .
1 | Page
Optical properties of (AR) multilayer thin film for solar cell application Fig.1.XRD Spectrum for the a) TiO2, b) TiO2-SiO2 and c) TiO2/SiO2 nano thin film prepared by hydrothermal method
3.2 UV Characterization The extrapolation graphs (Fig.3) indicate a direct optical transition and evaluated energy band gap of the prepared thin films. The optical band gap values of the, brookite type TiO 2-SiO2, TiO2/SiO2 thin film very slightly increased to 3.6eV and 3.8 eV [8-9]. The Fig.2 the blue shift of the absorption edge is observed that corresponds to the increase of the band gap (Eg) value for the TiO2, TiO2-SiO2, and TiO2/SiO2. TiO2 mixing with SiO2 (Fig.2) causes appearance of the absorption in the near visible spectral range due to the direct optical transition from valence band to conduction band.
Fig .2. UV Absorption and transmission spectrum for the hydrothermally prepared thin film
2 | Page
Optical properties of (AR) multilayer thin film for solar cell application
Fig.3. Optical band gap of the hydrothermally prepared thin film 3.2.1 Optical Properties The optical study of a solid concerns not only physical phenomena such as refraction, reflection, transmission, absorption, polarization, interference, of light but also the interactions of photon energy with matter and the consequent changes in the electron states. From reflection, transmission and absorption processes it is possible to evaluate the optical constants such as (1).Refractive index (n) and Absorption index or Extinction co-efficient (k),( 2). Thickness of the thin film (t), (3). Optical Band gap (Eg) and (4). Absorption coefficient (α). All these parameters were calculated by hydrothermally prepared thin films and tabulated, as seen in Table.2 [8-9]. TiO2-SiO2, TiO2/SiO2 Anti reflection coating layer is used in a solar cell, low reflectance should be confirmed.
Table.2. Calculated values of n, k, t and Eg for hydrothermally prepared thin films Samples
TiO2 SiO2 TiO2-SiO2 TiO2/SiO2
0.11878 0.0638 0.08077 0.1
Refractive index (n) 2.05178 1.675895 1.794079 1.924951
Extinction coefficient(k) 0.145318 0.763672 0.175334 0.66021
Thickness (t) 391.2 nm 4.17 μm 513.3 nm 254.0 nm
Optical Band gap Eg (eV) 3.44 1.46 3.6 3.8
3.3 Morphological Analysis The microstructure of the TiO2 nanoparticles synthesized by hydrothermal method in the present studied was observed by SEM which is shown in Fig.4. The prepared sample shows particle with great aggregation. The size of the particle is around 500nm. The shape of the particle is not uniform and it looks like spherical in shape. The microstructure of the thin film sample annealed at 300°C shows reduction in the agglomeration (Fig.4.c). The formed nanoparticles are visible clearly. Here also the shape of the particle was observed as sphere like morphology with different size around 230nm. (Fig.4d). shows that the size distribution is almost uniform compared to other particles and the size of the particle is almost 240nm. From the morphological analysis it is found that, the sample prepared by hydrothermal method improves the uniformity of the samples.
3 | Page
Optical properties of (AR) multilayer thin film for solar cell application
Fig.4.SEM image of a) & b) TiO2 c) TiO2-SiO2 and d) TiO2/SiO2 IV.
Synthesis and characterization of the photovoltaic materials (Nano structured of TiO2, SiO2, TiO2-SiO2 and TiO2/SiO2), is presented. The optical, structural, and morphological studies of the prepared thin films were analyzed. The optical band gap of the prepared TiO2-SiO2 and TiO2/SiO2 is slightly increases due to reduction of the particles size. Since the reflectance of the TiO2-SiO2 and TiO2/SiO2 is low, then the material are suitable for antireflection coating. Then the TiO2, SiO2, TiO2-SiO2 and TiO2/SiO2 thin film has good photocatalytic property. From the SEM, the uniformity of the particle size of TiO2-SiO2 and TiO2/SiO2 is higher than that of TiO2. The Srilankite structure is observed in the prepared TiO2 thin film. Brookite structure is also observed in the prepared TiO2-SiO2 and TiO2/SiO2 thin films. Hence, we can conclude that, hydrothermally prepared thin film shows better optical, structural, and morphological and photocatalytic property. Anti reflection coating layer of TiO2-SiO2 and TiO2/SiO2 is suitable for in a solar cell fabrication.
References: . . . . . . . . .
Mindaugas andrulevičius,sigitas tamulevičius, yuriy gnatyuk3, Nadija vityuk, natalia smirnova, anna eremenko, Mater.Sci.14,2008, 1. Abbas Hodroj,Odette Chaix-Pluchery, Marc Audier, Ulrich Gottlieb and Jean-Luc Deschanvres J .Mater.Res. 23, (3), 2008, 755. Jong-Gul Yoon, Hun Kyoo Oh and Young Jik Kwag, J.Kor. Phys. Soci. 33,(6),1998, 699-704. Emil Indrea, Anca Peter, Danut T Silipas, Simina Dreve, Ramona-Crina Suciu, Marcela Corina Rosu, Virginia Danciu and Veronica Cosoveanu, J. Phys. Conf. Series 182, 2009, 012066. F. Gracia , F. Yubero , J.P. Holgado , J.P. Espinos, A.R. Gonzalez-Elipe ,T. Girardeau, Else.Thin Solid Films 500 ,2006, 19 -26. A. Thangaraj, M.J. Eapen, S. Sivasanker, and P. Ratnasamy ZEOLITES, 12, 1992, 943-950. Jung Wook Lim, Sun Jin Yun, and Je Ha Kim, ETRI Journal, 31, (6), 2009, 675-679. A. SLAV, 6, ( 3), 2011, 915 – 920. Mindaugas ANDRULEVICIUS,Sigitas TAMULEVICIUS,Yuriy GNATYUK,Nadija VITYUK,Natalia SMIRNOVA,Anna EREMENKO, Mat.Sci.14,(1),2008,8-14.
4 | Page